Upload
ngomien
View
248
Download
5
Embed Size (px)
SHEAR STRENGTHENING OF PRE-CRACKED AND NON PRE-
CRACKED REINFORCED CONCRETE CONTINUOUS BEAMS USING BI-
DIRECTIONAL CFRP STRIPS
NOORWIRDAWATI BINTI ALI
A thesis submitted in
fulfillment of the requirement for the award of the
Doctor of Philosophy
Faculty of Civil and Environmental Engineering
Universiti Tun Hussein Onn Malaysia
SEPTEMBER 2014
v
ABSTRACT
Shear failure of a reinforced concrete beam is catastrophic where it occurs suddenly
and without any warning. The use of FRP sheet as a strengthening and repairing
material is an effective method to enhance the shear capacity of the beam. Extensive
researches have been conducted on the shear strengthening of reinforced concrete
simply supported beams using FRP composites. However, strengthening continuous
beams in shear have received very little attention among the researchers although
most of the existing structures are in the form of continuous condition. Furthermore,
there are restraints to add shear reinforcement to the existing reinforced concrete
beams when beams are part of the floor-beam system. In the design guideline by
ACI 440 Committee mentioned that the existing theoretical model have not been
confirmed to be use for strengthening in negative moment region which existed in
continuous beam. Therefore, in order to address the problem, a study on shear
strengthening of reinforced concrete continuous beam using CFRP strips was
conducted. An experimental work on 14 full-scale reinforced concrete continuous
beams with a size of 150x350x5800mm was carried out. Simulation using finite
element software ATENA v4 and theoretical analysis was also conducted. The
variables involved a number of CFRP strips layers (one and two layers), wrapping
schemes (four sides and three sides), orientation of CFRP strips (0/90 and 45/135
degree) and shear span to effective depth ratio, av/d (2.5 and 3.5). The type of FRP
used was bi-directional CFRP strips. Two beams were un-strengthened and treated
as the control specimens whilst the other 12 beam were wrapped with CFRP strips.
From the experimental results, all beams failed in shear as expected. Beams wrapped
with CFRP strips recorded shear capacity enhancement of around 10.12% to 53.74%
compared to the control specimens. Beam wrapped with two layers of CFRP strips at
four sides of the beam recorded the highest shear enhancement. Simulation study
also showed similar behaviour in terms of shear capacity and crack patterns. Three
existing theoretical models; ACI 440, Khalifa and Nanni and fib models were
adopted for theoretical comparison of shear capacity contributed by CFRP, Vf while
for shear capacity contributed by concrete, Vc and stirrups, Vs, the equation from
ACI 318-08, BS8110 and EC2 was adopted. The ACI 440 model had shown the
closer value with the experimental results and a modified ACI 440 model was
proposed on the effective strain limit and bond-reduction coefficient.
vi
ABSTRAK
Kegagalan ricih bagi rasuk konkrit bertetulang adalah merbahaya dimana ianya
berlaku secara tiba-tiba tanpa sebarang amaran. Penggunaan FRP sebagai bahan
pengukuhan dan pemulihan adalah satu kaedah yang telah diketahui efektif bagi
meningkatkan kekuatan ricih rasuk tersebut. Kajian yang mendalam telah pun
dilakukan ke atas pengukuhan ricih rasuk konkrit bertetulang disokong mudah.
Bagaimanapun, kajian ke atas pengukuhan ricih bagi rasuk selanjar masih tidak
mendapat perhatian yang meluas sedangkan kebanyakan struktur sedia ada adalah
dalam bentuk selanjar. Terdapat juga halangan bagi menambah tetulang ricih pada
rasuk konkrit bertetulang yang sedia ada apabila rasuk adalah sebahagian daripada
sistem papak-rasuk. Di dalam garis panduan rekabentuk yang dikeluarkan oleh ACI
440 Committee memberitahu bahawa model analitikal sedia ada masih belum
dipastikan bagi digunakan untuk pengukuhan rasuk dibahagian momen negatif yang
mana ianya wujud pada rasuk selanjar. Oleh itu, satu kajian telahpun dijalankan
terhadap pengukuhan ricih rasuk selanjar dengan menggunakan jalur-jalur CFRP.
Satu kajian makmal terhadap 14 rasuk selanjar konkrit bertetulang berskala penuh
dengan saiz 150x350x5800mm telahpun dijalankan beserta simulasi menggunakan
perisian unsur terhingga ATENA v4 dan analisis teori. Antara pembolehubah yang
terlibat ialah bilangan lapisan CFRP, skim balutan, orientasi jalur CFRP dan nisbah
rentang ricih terhadap kedalaman berkesan. Dua rasuk tidak diperkukuhkan dan
diambil sebagai rasuk kawalan manakala 12 rasuk yang selebihnya dibalut dengan
jalur-jalur CFRP. Daripada keputusan eksperimen, semua rasuk gagal dalam ricih
seperti yang telah dijangkakan. Rasuk yang diperkukuhkan dengan CFRP
mencatatkan peningkatan kekuatan ricih dalam lingkungan 10.12% - 53.74%. Rasuk
yang dibalut dengan dua lapis jalur CFRP mencatatkan peningkatan ricih yang
tertinggi. Kajian simulasi juga menunjukkan kelakuan yang sama dari segi kekuatan
ricih dan corak keretakan. Tiga model teori yang sedia ada iaitu ACI 440, Khalifa &
Nanni dan fib digunakan untuk perbandingan secara teori bagi kapasiti ricih oleh
CFRP, Vf manakala bagi kapasiti ricih oleh konkrit, Vc dan tetulang ricih, Vs, tiga
persamaan daripada ACI 318-08, BS8110 dan EC2 digunakan. Model ACI 440
menunjukkan nilai teori yang lebih hampir dengan ujikaji makmal dan satu
pengubahsuaian terhadap model tersebut telahpun dicadangkan ke atas had keterikan
berkesan dan pembolehubah pengurangan-ikatan.
vii
TABLE OF CONTENTS
TITLE i
DECLARATION ii
DEDICATION iii
ACKNOWLEDGEMENT iv
ABSTRACT v
ABSTRAK vi
TABLE OF CONTENTS vii
LIST OF TABLES xiii
LIST OF FIGURES xv
LIST OF SYMBOLS xxvi
LIST OF ABBREVIATIONS xxix
LIST OF APPENDIXES xxx
CHAPTER 1 INTRODUCTION
1.1 Introduction 1
1.2 Problem statement 2
1.3 Objective 3
1.4 Scope of study 4
1.5 Research significance 7
1.6 Structure of thesis 7
CHAPTER 2 LITERATURE REVIEW
2.1 Historical background of Fibre Reinforced Polymer 9
(FRP)
2.2 Advantages of FRP composites 10
2.3 Disadvantages of FRP composites 11
2.4 Fibre Reinforced Polymer constituents 11
2.4.1 Types of fibre reinforcement 12
2.4.2 Polymer matrix: Resins 14
viii
2.5 FRP application on structural member 15
2.6 Strengthening reinforced concrete structure using 16
FRP plate
2.7 Shear failure 18
2.7.1 Theory of shear 19
2.7.2 Behaviour of beams without stirrups 22
2.7.3 Factor affecting the shear strength of beams 23
without stirrups
2.7.4 Behaviour of beams with stirrups 28
2.8 Previous research on strengthening of RC beams 30
using FRP sheets
2.9 Factors affecting the contribution of the FRP sheets 39
to shear capacity
2.9.1 Wrapping schemes 39
2.9.2 Fibre orientation 40
2.9.3 End anchor 41
2.9.4 Biaxial reinforcement 42
2.9.5 Spacing of FRP strips 43
2.10 Theoretical models on the contribution of CFRP 44
sheets to shear capacity
2.10.1 Triantafillou model (1998) 44
2.10.2 Khalifa and Nanni model (2002) 45
2.10.3 ACI Committee 440 model (2008) 48
2.10.4 fib model (2001) 50
2.11 Numerical modeling of reinforced concrete 50
strengthened with FRP composites
2.12 Concluding remarks 57
CHAPTER 3 METHODOLOGY
3.1 Introduction 59
3.2 Specimens designation 59
3.2.1 Group 1 63
3.2.2 Group 2 63
3.2.3 Group 3 63
3.3 Test specification 64
ix
3.4 Material properties
3.4.1 Concrete 69
3.4.2 Reinforcement 70
3.4.3 Carbon Fibre Reinforced Polymer 71
3.5 Specimen preparation
3.5.1 Concrete mix 72
3.5.2 Formwork preparation 72
3.5.3 Reinforcement preparation 73
3.5.4 Casting of beam and curing 74
3.5.5 Installation of strain gauge
3.5.5.1 Installation on reinforcement 76
3.5.5.2 Installation on concrete surface 78
3.6 Instrumentation of test 79
3.7 Testing procedure 81
3.8 Finite element modelling
3.8.1 Introduction to ATENA (Advanced Tool for
Engineering Nonlinear Analysis 84
3.8.2 Material model
3.8.2.1 Concrete 84
3.8.2.2 Reinforcement 87
3.8.3 Mesh and boundary condition 88
3.8.4 Solution of nonlinear equations 89
CHAPTER 4 EXPERIMENTAL RESULTS
4.1 Introduction 91
4.2 Ultimate load 92
4.3 Modes of failure and crack pattern 97
4.3.1 Group 1 (initially strengthened beams with 98
av/d=2.5)
4.3.2 Group 2 (pre-cracked beams with av/d=2.5) 107
4.3.3 Group 3 (pre-cracked beams with av/d=3.5) 113
4.3.4 Key observation and discussion on the 123
ultimate load, modes of failure and crack pattern
4.4 Shear force – deflection (V- Δ) profile 125
x
4.4.1 Shear force – deflection profile of beams in 126
Group 1
4.4.2 Shear force – deflection profile of beams in 128
Group 2
4.4.3 Shear force – deflection profile of beams in 130
Group 3
4.4.4 Key observation and discussion on the 132
shear force – deflection profile
4.5 Shear force – strain relationship
4.5.1 Stirrups
4.5.1.1 Group 1 (initially strengthened beams 134
with av/d=2.5)
4.5.1.2 Group 2 (pre-cracked beams with 137
av/d=2.5)
4.5.1.3 Group 3 (pre-cracked beams with 138
av/d=3.5)
4.5.1.4 Influence of number of layer of CFRP 141
strips on stirrups
4.5.1.5 Influence of orientation of CFRP strips 144
on stirrups
4.5.1.6 Influence of wrapping schemes of CFRP 148
strips on stirrups
4.5.1.7 Influence of shear span to effective 156
depth ratio on stirrups
4.5.2 Concrete surface
4.5.2.1 Group 1 (initially strengthened beams 159
with av/d=2.5)
4.5.2.2 Group 2 (pre-cracked beams with 161
av/d=2.5)
4.5.2.3 Group 3 (pre-cracked beams with 163
av/d=3.5)
4.5.2.4 Influence of number of layer of CFRP 165
strips
4.5.2.5 Influence of orientation of CFRP strips 167
xi
4.5.2.6 Influence of wrapping schemes of 171
CFRP strips
4.5.2.7 Influence of shear span to effective 178
depth ratio
4.5.3 CFRP Strips
4.5.3.1 Group 1 (initially strengthened beams 180
with av/d=2.5)
4.5.3.2 Group 2 (pre-cracked beams with 183
av/d=2.5)
4.5.3.3 Group 3 (pre-cracked beams with 185
av/d=3.5)
4.5.3.4 Influence of number of layer of CFRP 187
strips
4.5.3.5 Influence of orientation of CFRP strips 189
4.5.3.6 Influence of wrapping schemes of 194
CFRP strips
4.5.3.7 Influence of shear span to effective 201
depth ratio
4.5.4 Comparison between stirrup, concrete surface 204
and CFRP strips.
4.5.5 Key observation and discussion on the shear 209
force-strain relationship of stirrups, concrete
surface and CFRP strips
CHAPTER 5 FINITE ELEMENT AND ANALYTICAL STUDY
5.1 Introduction 210
5.2 Finite element study 210
5.2.1 Load-deflection profile 211
5.2.2 Crack pattern 222
5.3 Analytical study 234
5.3.1 ACI 440 model 249
5.3.2 Khalifa and Nanni model 250
5.3.3 fib model 251
5.4 Analytical modeling 252
5.4.1 Influence of number of layer 252
xii
5.4.2 Influence of CFRP strips orientation 253
5.4.3 Wrapping scheme 253
5.4.4 Diagonal crack angle 255
5.4.5 Shear span to effective depth ratio 255
5.4.6 Proposed modified ACI 440 model 256
CHAPTER 6 CONCLUSIONS AND RECOMMENDATIONS
6.1 Summary 261
6.2 Conclusions 262
6.3 Recommendations 265
REFERENCES 267
APPENDIX A 273
APPENDIX B 278
APPENDIX C 284
xiii
LIST OF TABLES
2.1 Summary of strengthening of reinforced concrete beams 34
using FRP sheets
3.1 Details of specimens 61
3.2 Test requirement for each beam 68
3.3 Concrete cube compressive test results 69
3.4 Tensile test results of the reinforcement 71
3.5 Properties of SikaWrap-160 BI C/15 71
3.6 Properties of Sikadur-330 72
3.7 Default formula of concrete material parameters used in 86
ATENA
4.1 Experimental results of Group 1 94
4.2 Experimental results of Group 2 95
4.3 Experimental results of Group 3 96
4.4 Maximum deflection (at failure) 125
5.1 Comparison of experimental and simulation results of 212
ultimate load of beams in Group 1
5.2 Comparison of experimental and simulation results of 213
ultimate load of beams in Group 2
5.3 Comparison of experimental and simulation results of 214
ultimate load of beams in Group 3
5.4 Shear capacity (V) between theoretical value and experimental 236
results of beams in Group 1
5.5 Shear capacity (V) between theoretical value and experimental 237
results of beams in Group 2
5.6 Shear capacity (V) between theoretical value and experimental 238
results of beams in Group 3
5.7 Shear capacity contributed by concrete (Vc) between theoretical 239
value and experimental results of beams in Group 1
xiv
5.8 Shear capacity contributed by concrete (Vc) between theoretical 240
value and experimental results of beams in Group 2
5.9 Shear capacity contributed by concrete (Vc) between theoretical 241
value and experimental results of beams in Group 3
5.10 Shear capacity contributed by stirrups (Vs) between theoretical 242
value and experimental results of beams in Group 1
5.11 Shear capacity contributed by stirrups (Vs) between theoretical 243
value and experimental results of beams in Group 2
5.12 Shear capacity contributed by stirrups (Vs) between theoretical 244
value and experimental results of beams in Group 3
5.13 Shear capacity contributed by CFRP (Vf) between theoretical 245
value and experimental results of beams in Group 1
5.14 Shear capacity contributed by CFRP (Vf) between theoretical 246
value and experimental results of beams in Group 2
5.15 Shear capacity contributed by CFRP (Vf) between theoretical 247
value and experimental results of beams in Group 3
5.16 Shear capacity contributed by CFRP (Vf) between experimental 260
results and Proposed Modified ACI 440 model
xv
LIST OF FIGURES
1.1 Flow of research 6
2.1 Stress-strain relationship between CFRP, GFRP, AFRP and 13
steel reinforcement
2.2 Shear force and bending moment in a simply supported beam 19
2.3 A state of pure shear 20
2.4 Flexural and shear stresses 21
2.5 State of pure shear and principal stresses 21
2.6 Stress trajectories 21
2.7 Potential crack pattern 21
2.8 Shear mechanism acting in a beam without stirrups 22
2.9 The effect of shear span to effective depth ratio on shear 25
strength of beam without stirrups
2.10 Arch action 26
2.11 Types of failure 26
2.12 Shear-compression failure 27
2.13 Shear-tension failure 27
2.14 Diagonal-tension failure 27
2.15 Flexural failure 28
2.16 Crack categories 28
2.17 Distribution of internal shear in beam with shear reinforcement 29
2.18 Types of wrapping schemes for shear strengthening using 39
FRP laminates
2.19 Fibre orientation, θ = 90⁰ 40
2.20 Fibre orientation, θ = 0⁰ 40
2.21 Fibre orientation, θ = 45⁰ 41
2.22 End anchor 41
2.23 U-anchor system (after slicing a beam) 42
2.24 Uni-directional FRP sheet 42
xvi
2.25 Bi-directional FRP sheet 43
2.26 Vertical and inclined CFRP strips 43
2.27 Finite element model by Godat et. al (2007) 51
2.28 Meshing and boundary condition 53
2.29 Geometry meshing 54
2.30 Meshing of a beam 55
2.31 Finite element model of strengthened beam 56
2.32 Mesh of the shear-lap specimen 56
3.1 Organisation of specimens 62
3.2 Reinforcement details 65
3.3 Typical cross-section of the beams 65
3.4 Initially strengthen and repaired scheme for Group 1 and 66
Group 2 beams (av/d=2.5) with 0º/90º orientation of CFRP strips
3.5 Repaired scheme for Group 2 beams (av/d=2.5) with 45º/135º 66
orientation of CFRP strips
3.6 Repaired scheme for Group 3 beams (av/d=3.5) with 0º/90º 67
orientation of CFRP strips
3.7 Repaired scheme for Group 3 beams (av/d=3.5) with 45º/135º 67
orientation of CFRP strips
3.8 Concrete cube preparation 70
3.9 Concrete cube to be cured 70
3.10 Concrete cube after testing 70
3.11 SikaWrap-160 BI C/15 71
3.12 Sikadur-330 72
3.13 Plywood formwork 73
3.14 Steel formwork 73
3.15 Bending of links 74
3.16 Reinforcement cage 74
3.17 Process of pouring concrete into formwork and compaction 75
using mechanical vibrator
3.18 Curing of specimens 75
3.19 Specimen after detached from formwork 76
xvii
3.20 Strain gauge positions on reinforcement for beams with 77
av/d=2.5
3.21 Strain gauge positions on reinforcement for beams with 77
av/d=3.5
3.22 Final coating using self-bonding tape 78
3.23 Complete bonded strain gauge at the reinforcement 78
3.24 Strain gauge positions on concrete surface and CFRP for beams 79
with av/d=2.5
3.25 Strain gauge positions on concrete surface and CFRP for beams 79
with av/d=2.3
3.26 Test set-up for Group 1 and 2 (av/d=2.5) 80
3.27 Test set-up for Group 3 (av/d=3.5) 80
3.28 Process of placing specimen to Magnus Frame 81
3.29 Data Logger and LVDT attached to the tested specimen 81
3.30 Hydraulic control system 82
3.31 Marked surface on specimen 82
3.32 Grinding of concrete surface 82
3.33 Mixing of Part A and Part B of epoxy and final look of 83
mixed epoxy
3.34 Applying first and second layer of the epoxy 83
3.35 Applying CFRP to the specimen and rolled out the CFRP 84
to squeeze out the excess of epoxy
3.36 CFRP applied to the specimen 84
3.37 Stress-strain and biaxial failure law 87
3.38 The bilinear and multilinear stress-strain law for reinforcement 88
3.40 Concrete, steel plate and CFRP strips meshing 89
3.41 Boundary condition applied 89
4.1 Shear failure of Beam 1-0 at load 286.10kN (shear force 98
93.70kN)
4.2 Crack pattern of Beam 1-0 99
4.3 Shear failure of Beam 1-1 at load 379.68kN (shear force 100
124.35kN)
4.4 Crack pattern of Beam 1-1 101
xviii
4.5 Shear failure of Beam 1-2 at load 355.65kN (shear force 101
116.48kN)
4.6 Crack pattern of Beam 1-2 102
4.7 Debonding failure of CFRP strips for Beam 1-2 at load of 102
355.65kN (shear force 116.48kN)
4.8 Cracks on the top-side (crushing of concrete) of Beam 1-2 103
4.9 Shear failure of Beam 1-3 at load 439.86kN (shear force 104
144.05kN)
4.10 Stirrup failure of Beam 1-3 at load 439.86kN (shear force 104
144.05kN)
4.11 Shear failure of Beam 1-3 at load 439.86kN (shear force 104
144.05kN)
4.12 Crack pattern of Beam 1-3 105
4.13 Shear failure of Beam 1-4 at load 414.48kN (shear force 105
135.74kN)
4.14 Cracks along the cover of Beam 1-4 106
4.15 Crack pattern of Beam 1-4 106
4.16 Shear failure of Beam 2-1 at load 373.70kN (shear force 108
122.39kN)
4.17 Stirrup failure of Beam 2-1 at load 373.70kN (shear force 108
122.39kN)
4.18 Crack pattern of Beam 2-1 108
4.19 Shear failure of Beam 2-2 at load 338.08kN (shear force 109
110.72kN)
4.20 Crushing of concrete (top-side view) of Beam 2-2 109
4.21 Crack pattern of Beam 2-2 110
4.22 Shear failure of Beam 2-3 at load 411.25kN (shear force 111
134.68kN)
4.23 Crack pattern of Beam 2-3 111
4.24 Shear failure of Beam 2-4 at load 380.74kN (shear force 113
124.69kN)
4.25 Crack pattern of Beam 2-4 113
4.26 Crushing of concrete of Beam 3-0 114
xix
4.27 Shear failure of Beam 3-0 at load 253.65kN (shear force 114
86.24kN)
4.28 Crack pattern of Beam 3-0 115
4.29 Shear failure of Beam 3-1 at load 289.62kN (shear forcce 116
98.47kN)
4.30 Crack pattern of Beam 3-1 116
4.31 Beam 3-2 after pre-cracked phase 117
4.32 Shear failure of Beam 3-2 at load 279.32kN (shear force 118
94.97kN)
4.33 Crushing of concrete of Beam 3-2 118
4.34 Crack pattern of Beam 3-2 119
4.35 Shear failure of Beam 3-3 at load 325.39kN (shear force 119
110.63kN)
4.36 Stirrup failure of Beam 3-3 120
4.37 Crack pattern of Beam 3-3 120
4.38 Shear failure of Beam 3-4 at load 301.98kN (shear force 121
102.67kN)
4.39 Crushing of concrete of Beam 3-4 122
4.40 Crack pattern of Beam 3-4 122
4.41 Shear force – deflection graph of beams in Group 1 127
4.42 Shear force – deflection graph of beams in Group 2 129
4.43 Shear force – deflection graph of beams in Group 3 131
4.44 Shear force versus strain in stirrups for beams in Group 1 136
4.45 Shear force versus strain in stirrups for beams in Group 2 138
4.46 Shear force versus strain in stirrups for beams in Group 3 140
4.47 Shear force versus strain in stirrups between beam 142
wrapped with one layer and two layers of CFRP strips
(four sides wrapping scheme)
4.48 Shear force versus strain in stirrups between beam 143
wrapped with one layer and two layers of CFRP strips
(three sides wrapping scheme)
4.49 Shear force versus strain in stirrups between beam with 145
CFRP strips orientated at 0º/90º and 45º/135º
(four-side wrapping scheme) in Group 2
xx
4.50 Shear force versus strain in stirrups between beam with 146
CFRP strips orientated at 0º/90º and 45º/135º
(three-side wrapping scheme) in Group 2
4.51 Shear force versus strain in stirrups between beam with 147
CFRP strips orientated at 0º/90º and 45º/135º
(four-side wrapping scheme) in Group 3
4.52 Shear force versus strain in stirrups between beam with 148
CFRP strips orientated at 0º/90º and 45º/135º
(three-side wrapping scheme) in Group 3
4.53 Shear force versus strain in stirrups between beam with 150
CFRP strips at four sides and three sides of the beam
(initially strengthened with one layer of CFRP strips)
4.54 Shear force versus strain in stirrups between beam with 151
CFRP strips at four sides and three sides of the beam
(initially strengthened with two layers of CFRP strips)
4.55 Shear force versus strain in stirrups between beam with 152
CFRP strips at four sides and three sides of the beam
(pre-cracked beams with CFRP strips oriented at 0º/90º
orientation) in Group 2
4.56 Shear force versus strain in stirrups between beam with 153
CFRP strips at four sides and three sides of the beam
(pre-cracked beams with CFRP strips oriented at 45º/135º)
in Group 2
4.57 Shear force versus strain in stirrups between beam with 154
CFRP strips at four sides and three sides of the beam
(pre-cracked beams with CFRP strips oriented at 0º/90º)
in Group 3
4.58 Shear force versus strain in stirrups between beam with 155
CFRP strips at four sides and three sides of the beam
(pre-cracked beams with CFRP strips oriented at 45º/135º)
in Group 3
4.59 Shear force versus strain in stirrups for beams with 157
av/d=2.5 and av/d=3.5 (CFRP strips oriented at 0º/90º)
xxi
4.60 Shear force versus strain in stirrups for beams with 158
av/d=2.5 and av/d=3.5 (CFRP strips oriented at 45º/135º)
4.61 Shear force versus strain at concrete surface of beams 160
in Group 1
4.62 Shear force versus strain at concrete surface of beams 162
in Group 2
4.63 Shear force versus strain at concrete surface of beams 164
in Group 3
4.64 Shear force versus strain at concrete surface between beams 166
wrapped with one layer and two layers of CFRP strips
(four-side wrapping scheme)
4.65 Shear force versus strain at concrete surface between beams 167
wrapped with one layer and two layers of CFRP strips
(three-side wrapping scheme)
4.66 Shear force versus strain at concrete surface between beams 168
wrapped with CFRP strips at 0º/90º and 45º/135º orientation
(four-side wrapping scheme) – Group 2
4.67 Shear force versus strain at concrete surface between beams 169
wrapped with CFRP strips at 0º/90º and 45º/135º orientation
(three-side wrapping scheme) – Group 2
4.68 Shear force versus strain at concrete surface between beams 170
wrapped with CFRP strips at 0º/90º and 45º/135º orientation
(four-side wrapping scheme) – Group 3
4.69 Shear force versus strain at concrete surface between beams 171
wrapped with CFRP strips at 0º/90º and 45º/135º orientation
(three-side wrapping scheme) – Group 3
4.70 Shear force versus strain at concrete surface between beams 173
wrapped with CFRP strips at four and three sides of the beam
(one-layer strengthened beams)
4.71 Shear force versus strain at concrete surface between beams 174
wrapped with CFRP strips at four and three sides of the beam
(two-layer strengthened beams)
xxii
4.72 Shear force versus strain at concrete surface between beams 175
wrapped with CFRP strips at four and three sides of the beam
(0º/90º orientation – Group 2)
4.73 Shear force versus strain at concrete surface between beams 176
wrapped with CFRP strips at four and three sides of the beam
(45º/135º orientation – Group 2)
4.74 Shear force versus strain at concrete surface between beams 177
wrapped with CFRP strips at four and three sides of the beam
(0º/90º orientation – Group 3)
4.75 Shear force versus strain at concrete surface between beams 178
wrapped with CFRP strips at four and three sides of the beam
(45º/135º orientation – Group 3)
4.76 Shear force versus strain at concrete surface between beams 179
with av/d 2.5 and 3.5 (CFRP strips at 0º/90º orientation)
4.77 Shear force versus strain at concrete surface between beams 180
with av/d 2.5 and 3.5 (CFRP strips at 45º/135º orientation)
4.78 Shear force versus strain at CFRP strips for beams in Group 1 182
4.79 Shear force versus strain at CFRP strips for beams in Group 2 184
4.80 Shear force versus strain at CFRP strips for beams in Group 3 186
4.81 Shear force versus strain at CFRP strips between beams 187
wrapped with one layer and two layers of CFRP strips
(four-side wrapping scheme)
4.82 Shear force versus strain at CFRP strips between beams 188
wrapped with one layer and two layers of CFRP strips
(three-side wrapping scheme)
4.83 Shear force versus strain at CFRP strips between beams 190
wrapped with CFRP strips at 0º/90º and 45º/135º orientation
(four-side wrapping scheme) – Group 2
4.84 Shear force versus strain at CFRP strips between beams 191
wrapped with CFRP strips at 0º/90º and 45º/135º orientation
(three-side wrapping scheme) – Group 2
4.85 Shear force versus strain at CFRP strips between beams 192
wrapped with CFRP strips at 0º/90º and 45º/135º orientation
(four-side wrapping scheme) – Group 3
xxiii
4.86 Shear force versus strain at CFRP strips between beams 193
wrapped with CFRP strips at 0º/90º and 45º/135º orientation
(three-side wrapping scheme) – Group 3
4.87 Stress distribution for strengthened reinforced concrete beam 194
4.88 Shear force versus strain at CFRP strips between beams 196
wrapped with CFRP strips at four and three sides of the beam
(one-layer strengthened beams)
4.89 Shear force versus strain at CFRP strips between beams 197
wrapped with CFRP strips at four and three sides of the beam
(two-layer strengthened beams)
4.90 Shear force versus strain at CFRP strips between beams 198
wrapped with CFRP strips at four and three sides of the beam
(0º/90º orientation – Group 2)
4.91 Shear force versus strain at CFRP strips between beams 199
wrapped with CFRP strips at four and three sides of the beam
(45º/135º orientation – Group 2)
4.92 Shear force versus strain at CFRP strips between beams 200
wrapped with CFRP strips at four and three sides of the beam
(0º/90º orientation – Group 3)
4.93 Shear force versus strain at CFRP strips between beams 201
wrapped with CFRP strips at four and three sides of the beam
(45º/135º orientation – Group 3)
4.94 Shear force versus strain at CFRP strips between beams 202
with av/d 2.5 and 3.5 (CFRP strips at 0º/90º orientation)
4.95 Shear force versus strain at CFRP strips between beams 203
with av/d 2.5 and 3.5 (CFRP strips at 45º/135º orientation)
4.96 Shear force versus strain at stirrup, concrete surface and 206
CFRP strips of beams in Group 1
4.97 Shear force versus strain at stirrup, concrete surface and 207
CFRP strips of beams in Group 2
4.98 Shear force versus strain at stirrup, concrete surface and 208
CFRP strips of beams in Group 3
5.1 Shear force – deflection graph between experimental and 215
simulation results of Beam 1-0
xxiv
5.2 Shear force – deflection graph between experimental and 215
simulation results of Beam 1-1
5.3 Shear force – deflection graph between experimental and 216
simulation results of Beam 1-2
5.4 Shear force – deflection graph between experimental and 216
simulation results of Beam 1-3
5.5 Shear force – deflection graph between experimental and 217
simulation results of Beam 1-4
5.6 Shear force – deflection graph between experimental and 217
simulation results of Beam 2-1
5.7 Shear force – deflection graph between experimental and 218
simulation results of Beam 2-2
5.8 Shear force – deflection graph between experimental and 218
simulation results of Beam 2-3
5.9 Shear force – deflection graph between experimental and 219
simulation results of Beam 2-4
5.10 Shear force – deflection graph between experimental and 219
simulation results of Beam 3-0
5.11 Shear force – deflection graph between experimental and 220
simulation results of Beam 3-1
5.12 Shear force – deflection graph between experimental and 220
simulation results of Beam 3-2
5.13 Shear force – deflection graph between experimental and 221
simulation results of Beam 3-3
5.14 Shear force – deflection graph between experimental and 221
simulation results of Beam 3-4
5.15 The comparison of crack patterns at failure between 223
simulation and experimental results for Beam 1-0
5.16 The comparison of crack patterns at failure between 223
simulation and experimental results for Beam 1-1
5.17 The comparison of crack patterns at failure between 224
simulation and experimental results for Beam 1-2
xxv
5.18 The comparison of crack patterns at failure between 224
simulation and experimental results for Beam 1-3
5.19 The comparison of crack patterns at failure between 225
simulation and experimental results for Beam 1-4
5.20 The comparison of crack patterns between simulation 226
and experimental results for Beam 2-1
5.21 The comparison of crack patterns between simulation 227
and experimental results for Beam 2-2
5.22 The comparison of crack patterns between simulation 228
and experimental results for Beam 2-3
5.23 The comparison of crack patterns between simulation 229
and experimental results for Beam 2-4
5.24 The comparison of crack patterns at failure between 230
simulation and experimental results for Beam 3-0
5.25 The comparison of crack patterns between simulation 231
and experimental results for Beam 3-1
5.26 The comparison of crack patterns between simulation 232
and experimental results for Beam 3-2
5.27 The comparison of crack patterns between simulation 233
and experimental results for Beam 3-3
5.28 The comparison of crack patterns between simulation 234
and experimental results for Beam 3-4
5.29 Comparison of shear force capacity between experimental 248
results and theoretical value
5.30 Comparison of shear force contributed by CFRP strips 249
between experimental results and theoretical value
5.31 Comparison of shear force contributed by CFRP strips 257
between experimental results and theoretical value using
ACI 440 model
5.32 Comparison of shear force contributed by CFRP strips 259
between experimental results and theoretical value using
Proposed Modified ACI 440 model
xxvi
LIST OF SYMBOLS
⁰ Degree of angle
Ψ FRP strength reduction factor
Φ Strength reduction factor
γf Partial safety factor
α Angle of orientation of shear reinforcement
θ Angle of orientation of FRP reinforcement
β Angle of orientation of FRP reinforcement
ε Strain
εfu The ultimate strain in the FRP
εfe The effective strain in the FRP Δ Deflection
µ Micro
ρw Steel reinforcement ratio
ρf FRP reinforcement ratio
av/d Shear span to effective depth ratio
As Area of longitudinal tension reinforcement
As Area of shear reinforcement
Af The area of FRP shear reinforcement
Afv The area of FRP shear reinforcement
b Width of section
bw Web width
d Effective height of section
df The effective depth of FRP at section
Ef The modulus of elasticity of the FRP
I Moment of inertia
fx Flexural stress
fc’ Concrete compressive stress
fy Yield strength of longitudinal tension reinforcement
fv Yield strength of shear reinforcement
ffe The effective stress in the FRP
xxvii
ffu The ultimate stress in the FRP
Kv The bond-reduction coefficient
Kvm The modified bond-reduction coefficient
k1 Modification factor for concrete strength
k2 Modification factor for wrapping scheme
kN Kilo-Newton
Le The effective length of FRP reinforcement
nf Number of layer of FRP reinforcement
M Bending moment
Mu Factored moment at section
Pu,FEM Ultimate load of simulation results
Pu,exp Ultimate load of experimental results
s Spacing centre-to-centre between reinforcement
sf Spacing centre-to-centre between FRP strips reinforcement
tf Thickness of FRP sheet
v Shear stress
V Shear force
Vc Shear resistance of the uncracked concrete
Va Aggregate interlock force
Vd Dowel action
Vn Nominal shear strength
Vc Shear strength contributed by concrete
Vs Shear strength contributed by shear reinforcement
Vf Shear strength contributed by CFRP
Vcz Shear resistance of uncracked concrete
Va Interface shear transfer
Vus Ultimate shear strength of web steel
VRd The shear resistance of a member with shear reinforcement
Vfd The FRP contribution to shear capacity
Vu Factored shear force at section
VFEM Shear strength of simulation results
Vexp Shear strength of experimental results
Vtheory Shear strength of theoretical value
Vu Ultimate shear strength
xxviii
Vf,exp Shear strength of experimental results contributed by CFRP
Vf,theory Shear strength of theoretical value contributed by CFRP
wf Width of FRP strips
wfe The effective width of FRP strips
C1, C2, C3, C4 Strain gauge at concrete surface
F1, F2, F3, F4 Strain gauge at CFRP strips
S1, S2, S3, S4 Strain gauge at stirrups
xxix
LIST OF ABBREVIATIONS
2D Two dimensional
3D Three dimensional
ACI American Concrete Institute
AFRP Aramid Fibre Reinforced Polymer
ATENA Advanced Tool for Engineering Nonlinear Analysis
CEB The Euro-International Committee for Concrete
CFRP Carbon Fibre Reinforced Polymer
fib The International Federation for Structural Concrete
FIP The International Federation for Prestressing
FEM Finite Element Method
FRP Fibre Reinforced Polymer
GFRP Glass Fibre Reinforced Polymer
HFRP Hybrid Fibre Reinforced Polymer
LVDT Linear Variable Differential Transducer
N.A. Neutral Axis
TRC Textile Reinforced Concrete
UTM Universal Testing Machine
SBETA StahlBETonAnalyse (the analysis of reinforced concrete in German
language)
xxx
LIST OF APPENDIXES
APPENDIX A Design of specimen
APPENDIX B Calculation examples
APPENDIX C Comparison between the experimental results with the
theoretical values using effective strain from 0.0041 to
0.0045
1
CHAPTER 1
INTRODUCTION
1.1 Introduction In this few decades, the use of Fibre Reinforced Polymer (FRP) laminates as a
strengthening material has become a well known method in civil engineering.
However, prior to civil engineering, in the early days back to 1930s, FRP laminates
had been widely used in many areas such as aerospace, transportation, maritime and
electrical (ACI 440, 2006). In civil engineering, old buildings such as historical
building that need to be preserved are among the reasons why FRP has been widely
used. FRP laminates are chosen because of their good characteristics such as high
resistance to corrosion, high strength to weight ratio, ease of installation,
nonmagnetic, resistant to chemicals and high tensile strength. These advantages are
among the reasons FRP composites materials are an alternative solution to strengthen
existing structures (Chajes et al., 1995; Norris et al., 1997; Grace et al., 1998;
Khalifa & Nanni 2000; Taljsten 2003; Adhikary & Mutsuyoshi 2004;). Old
buildings and existing structures have motivated many researchers and organizations
to find alternative materials and techniques to restore the deteriorating and deficient
structures (Taljsten, 2003). In Malaysia, FRP laminates were used to streghthen and
repair the structure of the Middle Ring Road 2 (MRR2) in Kepong when the flyover
was seriously damaged and cracks were clearly seen at the piers and girders.
Past researches had shown great interest in shear and flexural strengthening
on reinforced concrete structures. Unlike flexural behaviour of cracked reinforced
concrete beams which can be well predicted, the prediction of shear behaviour of
reinforced concrete beams is a tough task due to its complexity on shear transfer
mechanism (El-Ariss, 2007). Bank (2006) pointed out that the preferable modes of
2
failure in a reinforced concrete beam is yielding of the tension reinforcement and
followed by crushing of the concrete in the compression zone.
Shear resistance of a reinforced concrete beams is a contribution from the
shear transfer in the compression zone, aggregate interlock across the crack face,
stirrups crossing the shear crack and the dowel action of longitudinal reinforcing bars
crossing the crack in the concrete. The shear failure of reinforced concrete beam
could be by diagonal tension failure or shear compression failure (Balaguru et al.,
2009). In order to strengthen or repair structure with shear defect, composites
materials have been widely used. For shear strengthening using composite materials,
the composites can be in many forms which include sheets, plates or bars along the
depth of the beam or perpendicular to the potential shear cracks. Shear strengthening
has also been found to improve the ductility because of the partial confining provided
by the strengthening systems (Balaguru et al., 2009).
1.2 Problem statement Structures that fail in shear are more dangerous than flexural failure because shear
failure occurs suddenly and without any warning (Khalifa & Nanni, 2000, Zhang and
Hsu, 2005; Jayaprakash et al., 2008). Shear failure is a diagonal tension failure that
is brittle in nature and should be avoided (Wang et al., 2007) The behaviour of
reinforced concrete in shear is very complex as the current code and design
procedures are based on analysis of experimental results and model assumption
rather than on an exact universally acceptable theory. The complexion is due to the
non-homogeneity of material, nonlinearity of material, cracks, presence of
reinforcement, load effects and the environment (Pillai et al., 1999).
Therefore, it is important to strengthen a structure that is deficient in shear.
Khalifa & Nanni (2000) observed that many existing reinforced concrete structures
are deficient in shear and are of need to be repaired. Reasons for these deficiencies
are insufficient shear reinforcement, increase of service load and corrosion of the
reinforcement. Historically, the strengthening and repairs of existing concrete
structures have been done by using conventional techniques such as external bonded
steel plates, steel or concrete jackets and external post-tensioning (ACI Committee
440, 2002). However, these conventional techniques require maintenance where a
3
steel plate has the risk of corrosion due to the environment. As this problem arises, a
lot of studies have been carried out to find a solution to overcome the problem.
Generally, most of investigations carried out experimentally by previous
researchers focused on shear strengthening of reinforced concrete beams that are
simply supported. In reality, the existing model has not been confirmed for shear
strengthening in areas subjected to combine high flexural and shear stresses or in
region of negative moment (ACI Committee, 2008), whereas most of existing beams
are in the form of continuous condition. Furthermore, there are restraints to add
shear reinforcement to existing reinforced concrete beams when beams are a part of
floor-beam system. For that reasons, FRP has been seen as the solution to overcome
the problems. Therefore, an application of composites material has been emphasized
to extend the service life of existing concrete structures. In this research, in order to
fill the gap, 14 continuous beams strengthened and repaired using CFRP strips have
been casted and tested where the results were then analyzed and compared with
simulation and theoretical study.
1.3 Objective The main aim of this study was to investigate the effectiveness of using externally
bonded bi-directional Carbon Fibre Reinforced Polymer (CFRP) composites as a
shear strengthening and repair technique for reinforced concrete continuous beams.
At the end of the research work, a theoretical model for the shear capacity of these
beams is expected to be established. To ensure the success of this research work, the
following objectives were outlined:
a) To investigate the shear behaviour of externally bonded reinforced concrete
continuous beams using CFRP strips with different parameters such as shear
span to effective depth ratio, number of layer, wrapping scheme and
orientation of CFRP strips.
b) To compare and validate a finite element model of reinforced concrete
continuous beams strengthened and repaired using CFRP strips with the
experimental results.
4
c) To propose a modified empirical equation for the shear strength contribution
of CFRP (Vf) for reinforced concrete continuous beams externally bonded
with CFRP strips.
1.4 Scope of study This study focused on shear strengthening and repair of reinforced concrete
continuous beam using externally bonded CFRP sheet. Therefore, in order to
achieve the above-mentioned objectives, the following scopes and limits were
outlined:
i) Conducting an experimental work on two-span continuous beams with a size
of 150mm width, 350mm depth and 5800mm of total length.
ii) All specimens were designed to fail in shear. Sufficient flexural
reinforcement was employed on the specimens to avoid any failure due to
flexure.
iii) A total of 14 specimens were casted and tested including two control
specimens and 12 reinforced concrete beams strengthened and repaired with
different schemes of CFRP strips.
iv) The specimens were divided into two groups of different shear span to
effective depth ratio (av/d) i.e. 2.5 and 3.5 respectively.
v) All specimens had identical design detail with similar concrete compressive
strength of 30N/mm², main reinforcement tensile strength of 460N/mm2 and
stirrups tensile strength of 250N/mm2.
vi) The bi-directional CFRP sheet was selected for the experimental programme.
vii) The width of the CFRP strips was selected at 80mm, whilst the spacing
between strips was located at 150mm centre to centre.
viii) The parameter involves shear span to effective depth ratio, number of layer,
wrapping scheme and orientation of CFRP strips.
ix) The experimental performance observation consisted of the deflection of the
specimen, ultimate load, loading history, strain of stirrup, concrete surface
and CFRP strips as well as modes of failure and crack pattern of the
specimens.
5
x) The simulation using of finite element analysis software (ATENA V4) was
conducted to analyze the theoretical behaviour of the specimens, to compare
and the results were then verified using the experimental results obtained.
Figure 1.1 shows the flow chart of the research work conducted. Initially, a
literature review was carried out focusing on the background of the CFRP
composites, shear strengthening of reinforced concrete continuous beams and the
theoretical modelling from previous researchers. This was followed by a series of
laboratory work encompassing the fabrication and instrumentation of the continuous
beams. This step also involved the installation of CFRP strips as well as testing
procedure of the continuous beams. Upon completion of the laboratory work, an
analysis of the data collected from the testing procedure was conducted. The data
were then compared with the theoretical investigation from the computational study
using finite element software (ATENA V4). Finally, an empirical equation for the
shear capacity of strengthened and repaired reinforced concrete continuous beams
using externally bonded CFRP composites were established.
6
Figure 1.1: Flow of research
Proposing a modified empirical equation for shear capacity of continuous beam strengthened
using CFRP strips
Ultimate load and
crack pattern
Shear force –
deflection profile
Shear force – strain
behaviour
Simulation study using ATENA V4
software
Experimental Program
Application of External CFRP Reinforcement
Theoretical Investigation
Finite Element Model
Three existing model: ACI 440, Khalifa & Nanni
and fib
Testing of reinforced concrete continuous beams with av/d=2.5
and 3.5
Comparison and validation of experimental results with finite element and existing theoretical
models
7
1.5 Research significance FRP composites as strengthening and repairing materials have been acknowledged as
an effective method to increase the load capacity of reinforced concrete beams. This
was proved from extensive studies done by many researchers (Chajes et al.,1995;
Hollaway & Leeming, 1999; Khalifa & Nanni, 2002; Zou, 2003; Taljsten &
Blanksvard, 2007; Jayaprakash et al., 2008). Most of the studies focused on
strengthening of un-cracked reinforced concrete beam and limited studies were done
on repair of defected or cracked reinforced concrete beam. However, Jayaprakash et
al., (2008) had conducted an experimental work on strengthening un-cracked
reinforced concrete simply supported beam and repair of pre-cracked reinforced
concrete simply supported beam. Their findings revealed that the pre-cracked beam
could perform as good as the initially strengthened beam due to the presence of
CFRP sheet.
The current design codes on strengthening using FRP composites were
developed based on experimental results of un-cracked reinforced concrete beam (fib,
2001; ACI Committee 440, 2008). Therefore, more experimental data on repair of
cracked reinforced concrete beam are needed to verify the design codes to be applied
on cracked reinforced concrete beam. As mentioned in the problem statement of this
study, shear strengthening in negative moment region has not been confirmed by the
current design code by ACI Committee 440 (2008). Therefore, in order to fill the
gap on strengthening and repairing of cracked reinforced concrete beam and shear
strengthening in negative moment region, this study which was focusing on shear
strengthening and repair of un-cracked and pre-cracked reinforced concrete
continuous beam was conducted. An experimental work followed by simulation
study using finite element software (ATENA V4) and theoretical analysis was
executed where a modification on the current design code by ACI Committee 440
was proposed.
1.6 Structure of thesis Chapter 1 presents an introduction to the thesis including the problem statement,
objectives, scope of research and the significance of this research.
8
Chapter 2 reviews previous research work on shear strengthening and repair of
reinforced concrete beams externally bonded with Carbon Fibre Reinforced Polymer
(CFRP) strips. In-depth study on the existing theoretical models for the prediction of
the shear capacity of the strengthened beams was also reviewed.
Chapter 3 presents the research methodology of experimental work on 14 reinforced
concrete continuous beams strengthened and repair using CFRP strips. This chapter
also presents the material properties, specimen preparation and test set-up and
instrumentation. This chapter also presents the methodology of finite element
modeling using ATENA v4 software.
Chapter 4 presents the experimental results of shear strengthening of reinforced
concrete continuous beams using CFRP strips. The data analysis includes the
discussion on ultimate load, crack pattern, shear force – deflection profile and shear
force – strain behaviour. The strain was observed on stirrups, concrete surface and
CFRP strips.
Chapter 5 presents the simulation results and its validation of the experimental data.
In addition, this chapter also shows the theoretical values using three existing model;
ACI 440, Khalifa & Nanni and fib model. Comparison between experimental results
and theoretical values was also discussed. Finally, a modified empirical equation on
shear strength contribution of CFRP for continuous beams was proposed.
Chapter 6 summarizes the experimental, simulation and theoretical result. This
chapter concludes the major findings of the research and proposed recommendation
for future research.
9
CHAPTER 2
LITERATURE REVIEW
2.1 Historical background of Fibre Reinforced Polymer (FRP)
The use of basic materials in the fabrication of dwellings including mud, straw, wood
and clay had been widely used in the early ages. While the concept of composites
has been in existence for several millennia, the incorporation of Fibre Reinforced
Polymer (FRP) composites technology into the industrial world is less than a century
old. The true age of plastics emerged just after 1900, with chemists and industrialists
taking bold steps to have plastics (vinyl, polystyrene, and plexiglass) mimic and
outdoor natural materials. The first known FRP product was a boat hull
manufactured in the mid-1930s as part of a manufacturing experiment using a
fibreglass fabric and polyester resin laid in a foam mold (ACI Committee 440, 2006).
From this first invention, FRP has been widely used in many areas and industries
such as aerospace, marine, transportation and electrical due to its extraordinary
strength and stiffness properties.
One of the advantages of using FRP is its corrosion-resistance characteristic
which contributes to its tremendous used in the US Air Force and Navy arena. In
1960s, the British and U.S. naval forces developed minesweeper ships using FRP
composites, as these materials are superior in aggressive marine environment and are
non-magnetic in nature (ACI Committee 440, 2006). Since that, FRP has received an
extensive attention among the researchers to develop new products by using FRP as
part of the materials. In recent years, the benefit of FRP composites especially
corrosion resistance characteristics has contributed to its application in the public
sector.
10
While the majority of the historical and durability data of FRP composite
installations comes from the aerospace, marine and corrosion resistance industries;
FRP composites have been used as a construction material for several decades. FRP
composite products were first demonstrated to reinforce concrete structures in the
mid-1950s (ACI Committee 440, 2006). Due to its excellent performance, the use of
FRP was expanded to restore historic buildings and other structural applications.
2.2 Advantages of FRP composites
FRP composites have many advantages such as good corrosion resistance, light
weight, high strength to weight ratio, easy to install, non conductive and resistance to
the chemicals (Triantafillou & Antonopoulus, 2000). Apart from the defense area,
FRP composites also provide many advantages in civil engineering. With many
serious problems such as the service life of the structures, corrosion of reinforcement,
design faults and improper planning, FRP is believed to be one of the solutions.
The bonding of FRP plate on the tensile face has been proven to be an
effective method to increase both the strength and stiffness of concrete members
(Leung & Pan, 2005). Depending on the products and applications, FRP materials
for civil infrastructure or construction applications can be optimized for specific load.
Besides that, reduced dead load of FRP components of rehabilitated structures can
result in increased load ratings. The use of FRP also reduces the maintenance costs
because of resistance to deicing salts and other corrosive agents (ACI Committee
440, 2006). The other advantages of FRP composites are; they can reduce field
installation time by using engineered system packaging, reduce traffic delays because
of the faster construction, increase reliability by pre-engineered systems, enhance the
durability and fatigue characteristics and increase the service life of the structure.
Besides that, because on the innovative and efficient installations, the engineering
value of the products and systems are improved (ACI Committee 440, 2006).
11
2.3 Disadvantages of FRP composites
Using FRP composites has its disadvantages. Taljsten & Blanksvard (2007)
highlighted that since the application of FRP in building industries has been around
only for 10 years, there were insufficient data to verify that FRP has good long-term
properties. The working environment while handling FRP composites is also
important as any mishandling of these materials may cause injuries to workers. FRP
composites have low ductility where the stress-strain relationship is linear that could
cause a sudden and brittle failure (Kodur & Baingo, 1998).
2.4 Fibre Reinforced Polymer constituents
Fibre Reinforced Polymer is a composite material, tailored by a large number of thin
high strength fibres embedded in a plastic resin (ACI Committee 440, 2006). FRP is
defined as a polymer matrix, either thermoset or thermoplastic, that is reinforced with
a fibre or other reinforcing material with a sufficient aspect ratio (length-to thickness)
to provide a discernible reinforcing function in one or more directions (ACI
Committee 440, 2006). Cusson & Xi (2002) have stated that a fibre-reinforced
polymer or FRP is an advanced composite or material system. It is defined as a solid
material which is composed by two or more substances having different physical
characteristics in which each substance retains its identity while contributing
desirable properties. It is also a structural material made of plastic within which a
fibrous material is embedded; the components remain physically identifiable
exhibiting an interface between one another.
Fibres are characterized by an excellent tensile strength in the direction of the
fibres and negligible strength in the transverse direction. These fibres are named as
uni-directional fibre system. The woven or bi-directional fabrics are made up of
fibres oriented at both 0 degree and 90 degree with an equal distribution of fibres in
each direction. There are many types of FRP composites based on the modifiers used
such as Glass Fibre Reinforced Polymer (GFRP), Carbon Fibre Reinforced Polymer
(CFRP), Aramid Fibre Reinforced Polymer (AFRP) and Hybrid Fibre Reinforced
Polymer (HFRP) for composites containing different types of fibres (ACI Committee
440, 2006). The major differences between the FRP composite reinforcement and
12
steel reinforcement are that the FRP has higher elastic strength, lower stiffness and
elastic behaviour up to failure without any yielding plateau.
The performance of any composite depends on the materials of which the
composite is made of, the arrangement of the primary load-bearing portion of the
composite (reinforcing fibres) and the interaction between the materials (fibres and
matrix) (ACI Committee 440, 2006). In general, FRP composite is made by the
combination of fibres and polymer resin where the polymer resin surrounds and
binds the fibres together. The resin influences the physical properties of the end
product while the fibres provide the mechanical strength. Fillers and additives are
used to impart special properties to the end product.
2.4.1 Types of fibre reinforcement
In civil engineering, there are three types of fibres commonly used; glass, carbon and
aramid. The fibre component consists of fine thread-like natural or synthetic material
characterized by its aspect ratio (fibre length divided by fibre diameter) and width
length nearly 100 times its diameter (Cusson & Xi, 2002). Glass fibres are produced
by extruding molten mass through an orifice of 0.79-3.18mm in diameter followed
by drawing through fine opening of 3-20µm in diameter (ACI Committee 440, 2006).
Glass fibres are commercially available in E-glass formulation (for electrical grade),
the most widely used general purpose form of composite reinforcement and other
formulations for high strength (S-2 glass), improved acid resistance (ECR glass) and
alkali resistance (AR glass) (ACI Committee 440, 2006). The advantage of glass
compared to carbon and aramid is it is a good impact-resistant fibre. However, glass
is denser than carbon and aramid. The end product of glass fibre is a good electrical
and thermal insulation materials. Apart from that, glass fibre is also used for radar
antenna applications due to its characteristic which is transparent to radio frequency
(ACI Committee 440, 2006).
Carbon fibres are also known as graphite fibres. Three natural resources
supply the production of structural carbon fibres: pitch, a product of petroleum
distillation; PAN, polyacrylonitrile and rayon (Cusson & Xi, 2002). The properties
of carbon fibres are controlled by molecular structure and degree of freedom from
defects. The formation of carbon fibres requires processing temperatures of above
13
1000°C (1830°F) (ACI Committee 440, 2006). High strength, high strength to
weight ratio, low longitudinal and transverse coefficient of thermal expansion, low
sensitivity to fatigue loads and excellent moisture and chemical resistance are some
of the advantages of carbon fibres. Carbon fibre is about five to ten times more
expensive than glass fibre. However, it has about twice the usable strength and four
times the modulus of glass (ACI Committee 440, 2006).
The aramid or aromatic polyamide fibres are manufactured by extruding
polymer solution through a spinneret resulting in a fibre with high thermal stability,
high strength and high stiffness. The aramid fibres are fire resistant and perform well
at high temperatures. The tensile strength of aramid fibres is higher than that of glass
fibres and the modulus is about 50% higher (ACI Committee 440, 2006). The other
advantages of aramid fibres are resistant to organic solvents, fuels and lubricant,
increase the impact resistance of composites and they are also a good insulator of
electricity and heat. However, aramid composites have poor compressive strength
and composites using such aramid fibres should be carefully designed, especially for
compression or bending (ACI Committee 440, 2006). Figure 2.1 shows the stress-
strain relationship between CFRP, GFRP, AFRP and steel reinforcement (Khalifa,
1999).
Figure 2.1: Stress-strain relationship between CFRP, GFRP, AFRP and steel
reinforcement (Khalifa, 1999)
14
2.4.2 Polymer matrix: resins Resins can be classified into two groups: thermosetting and thermoplastic (ACI
Committee 440, 2006). Thermoset resins are liquids or low melting point. They are
cured with a catalyst, heat or a combination of the two. Once thermoset resins are
cured, they cannot be converted back to their original liquid form. Cured thermoset
will not melt and flow but it will soften when heated (ACI Committee 440, 2006).
For thermoplastic resins, they can be repeatedly softened at high temperature.
Thermoplastic resins become soft when heated and may be shaped or molded while
in a heated semi-fluid state and vice versa, they become rigid when cooled (ACI
Committee 440, 2006). Thermoset resins are used for structural purposes for their
ability to undergo a chemical reaction when cured (Cusson & Xi, 2002). The most
common thermosetting resins used in composites are polyesters, epoxies, vinylesters
and phenolics.
Polyesters are versatile because of their capacity to be modified or tailored
during the building of the polymer chains. The principal advantage of these resins is
a balance of properties (including mechanical, chemical and electrical) dimensional
stability, cost and ease of handling or processing (ACI Committee 440, 2006).
Epoxy resins are the most widely used and accepted as structural adhesive available
commercially since 1940s. Epoxy resins are used with a number of fibrous
reinforcing materials, including glass, carbon and aramid (ACI Committee 440,
2006). It has the ability to produce a continuous bond between fibre reinforced
polymer (FRP) and concrete to ensure that full composite action is developed by the
transfer of shear stress across the thickness of the adhesive layer.
Vinylesters are developed to combine the advantages of epoxy resins with
those of unsaturated polyester resins (ACI Committee 440, 2006). The advantages of
vinylesters are they offer mechanical toughness and excellent corrosion resistance.
The process of fabricating vinylesters is not as complex as epoxy resins (ACI
Committee 440, 2006). Vinylester resins tend to saturate the fibres more efficiently
resulting in higher strength, while epoxies require much higher fibre content.
Vinylesters also bond well to glass to increase the resistance of these fibres in
aggressive chemical environments (Cusson & Xi, 2002).
Phenolics are a class of resins commonly used on phenol (carbolic acid) and
formaldehyde and cure through a condensation reaction producing water that must be
15
removed during processing (ACI Committee 440, 2006). The advantages of
phenolics resins include high temperature resistance, creep resistance, excellent
thermal insulation and sound damping properties and corrosion resistance (ACI
Committee 440, 2006). However, phenolics resins are not widely used for the
construction industry. They are applied as a binder in engineered wood, brake
linings, clutch plates and circuit boards.
2.5 FRP application on structural member
FRP applications have been widely used in civil engineering arena. Bank (2006) has
mentioned that the used of FRP for new structural members could be divided into
three; (1) FRP bars or grid reinforced concrete members, (2) FRP tendons for pre-
stressed concrete members and (3) stay-in-place FRP formwork for reinforced
concrete members. However, the applications of FRP for existing structural
members are divided into two major types i.e. strengthening and repair. FRP
strengthening means the increase of original design structure’s capacity and strength
while repair is where FRP is used to retrofit an existing and deteriorated structure
allowing its strength and capacity back to its original design.
FRP bars are used as an alternative material to steel reinforcement when
subjected to potential corrosion condition. FRP bars are commonly used in severe
environmental condition such as coastal environments and water treatment plants. It
includes dry-docks, sea walls, wharfs, box culverts, reinforced piles, floating piers,
tank, facades and retaining walls (Gravina & Smith, 2008). El-Sayed & Soudki
(2011) highlighted the use of FRP bars as the main reinforcement for reinforced
concrete members where magnetic transparency is required. Many studies on bond
characteristic between FRP bars and concrete, its ductility behavior of FRP and
moment distribution of members with FRP bars have also been widely covered by
other researchers.
FRP tendons are used as an alternative material to steel tendons. FRP tendon
has high tensile strength in the direction of the fibres and weak in the transverse
direction (Elrefai et al., 2006). Zou (2003) mentioned, using FRP tendon in concrete
members is the perceived reduction in ductility due to FRPs linear stress-strain
relationship up to failure and its relatively low strain at rupture. The advantages of
16
using FRP tendons include their non-corrosive and non-conductive properties,
lightweight and high tensile strength. Therefore, in the last few decades, the
application of FRP tendons was widely used in the construction of concrete bridges
(Youakim & Karbhari, 2006).
The use of stay-in-place FRP formwork is a system that acts to reinforce the
concrete after it has been cured (Bank, 2006). FRP stay-in-place (SIP) form has been
considered as an alternative to steel SIP form that can reduce the construction cost
and time. This is due to the reduced of transportation requirements and ease of
construction where it is light in weight (Hanus et al., 2008). FRP tubular SIP forms
have also been used to manufacture beam and column members where they are also
referred to as concrete-filled FRP tubes (Bank. 2006).
Strengthening reinforced concrete structure using FRP material is a technique
to increase the load and displacement capacity of a member. This is to make the
structure compatible with current existing building codes and regulations or due to
the changes in the use of the structure itself (Bank, 2006). There are a few types of
strengthening using FRP which include strengthening using externally bonded FRP
sheets and plates. The research on strengthening existing structure has been widely
explored by many researchers since the application of FRP to replace steel plate as a
strengthening material has been found to give better results in terms of corrosion
resistance.
The strength and ductility of damaged structures of existing reinforced
concrete structures due to corrosion, design failure or seismic impact can be
increased through repair and rehabilitation processes using FRP. Rehabilitation of
historical buildings is required because of its special characteristics and historical
reasons. FRP is used because it is more suitable and superior than other types of
materials as RFP is lightweight, has high strength and has better corrosion resistance.
2.6 Strengthening reinforced concrete structure using FRP plate
FRP composites such as FRP bar, FRP sheets as well as FRP plates have been used
to strengthen reinforced concrete structures. The use of FRP plates has contributed
in structural deficiencies. For example, replacement of steel reinforcement by plates
may lead to corrosion due to the environment, adding tensile element of inadequate
17
flexural capacity of reinforced concrete using FRP plates, adding FRP plate to the
tensile face to avoid of sudden failure and externally bonded stressed plates or web
reinforcement to enhance shear capacity of reinforced concrete element. Hollaway &
Leeming (1999) have highlighted some of the advantages using FRP plate bonding as
a means for strengthening existing structures:
i) The ultimate strength of FRP plates can be varied to meet different
requirement of the strengthening schemes needed.
ii) FRP plate has a density of only 20% from the density of steel and therefore
the weight of FRP plate is lighter than the steel plate. This could save cost for
transportation as well as installation. FRP plates do not require concrete
jacket as compared to steel plate.
iii) The weight of FRP plate is low and it can be easily transferred by a single
man at the site. Transporting these materials only require light vehicles
without the need of lorries for delivery.
iv) FRP plate has a versatile design system compared with steel plate. The work
of bonding can be done at site while steel plates are limited in length and in-
situ welding may not be possible.
v) Compared to steel plates, FRP plates are more durable because they do not
corrode due to the environment. The corroded steel plates could reduce the
long term performance of the steel plates itself.
vi) Another advantage of FRP is due to its low conductivity of heat compared to
steel, FRP plates have good resistance to fire.
vii) FRP plates do not need maintenance while steel plate will require constant
monitoring and maintenance.
Despite its advantages, FRP plates also have some disadvantages. The disadvantages
of FRP plates as highlighted by Hollaway & Leeming (1999) are as follows:
i) Fibre reinforced composites are an expensive material compared to steel
plates. However, it is predicted that the difference of price between the two
materials is expected to be reduced because of the possible increase in
production.
18
ii) FRP plates are easily damaged by sharp objects. Compared with steel plates,
the damage of FRP plates is more likely to be localized as the plate is thinner
and more flexible.
2.7 Shear failure The study on shear failure has received great attention among researchers on every
aspect such as factors contributing to shear failure and design aspect. Generally,
shear failure is a diagonal tension failure that is brittle in nature and should be
avoided (Wang et al., 2007). In these few decades, using FRP is one of the solutions
to overcome shear failure problems and since then research using FRP for shear in
strengthening on structural members has been extensively conducted.
Due to the differences in mechanical properties between FRP and steel
reinforcement, particularly the modulus elasticity, the shear strength of concrete
members reinforced longitudinally with FRP bars may differ from that of members
reinforced with steel. Although there is a guideline by ACI Committee 440 about the
shear design for structures reinforced with FRP, many researchers have conducted
further studies on the shear design provisions. ACI Committee 440 has
recommended that the shear design for reinforced concrete beams reinforced with
FRP are based on the design formulas of members reinforced with conventional steel.
ACI is currently in the process of revising its approach to the calculation of the
concrete contribution to shear resistance of FRP reinforced concrete members.
Current design guidelines generally follow the format of conventional
reinforced concrete design methods (Razaqpur et al., 2006). The test results from the
investigation revealed that concrete shear strength of concrete beams reinforced with
FRP bars to that of beams reinforced with steel is proportional to the cube root of
axial stiffness ratio between FRP and steel reinforcing bars. The higher the
reinforcement ratio or modulus of elasticity of the reinforcing bars, the higher the
shear strength is obtained.
19
2.7.1 Theory of shear
Shear failure of reinforced concrete occurs due to a combination of stresses resulting
from the applied shear force, bending moments and sometimes axial load as well as
torsion. The behaviour of reinforced concrete in shear is very complex as the current
code and design procedures are based on the analysis of experimental results and
model assumption rather than on the acceptable theory. The complexity are due to
the non-homogeneity of material, nonlinearity of material, cracks, presence of
reinforcement, load effects and many other things (Pillai et al., 1999).
Shear cracks are developed due to principal tensile stresses exceeding the
tensile strength of the concrete (MacGregor & Bartlet, 2000). For the simple beam
as shown in Figure 2.2, the bending moment M at section A-A causes compressive
stresses in the concrete above the neutral axis (N.A) and tensile stresses in the
reinforcement as well as concrete below the neutral axis. An element located at the
neutral axis generates a state of pure shear as shown in Figure 2.3 where there are no
tensile or compressive stresses on the faces of the element and acting on 45º plane.
This diagonal tension causes diagonal cracking, thus the failures in beams commonly
referred to as ‘shear failures’ are actually tension failures at the inclined cracks
(Wang et al., 2007).
A A N.A M
V A A
Figure 2.2: Shear force and bending moment in a simply supported beam (Wang, et al., 2007)
20
(Equation 2.2)
(Equation 2.1)
v ft(max) = V v v V 45º v v
Figure 2.3: A state of pure shear (Wang et al., 2007)
For a homogeneous rectangular concrete beam, the flexural stress, fx and shear stress,
v at a point in the section distant y from the neutral axis are given by:
푓 = 푀푦퐼
푣 =
where:
Q = The first moment of the area of section above the depth y,
about the neutral axis = Ay
I = Moment of inertia of the section
Figures 2.4 to 2.7 show the flexural and shear stresses, principal stresses, stress
trajectories and potential crack pattern of a simply supported beam respectively
(Pillai et al., 1999). Concrete cracks when the principle tensile stresses exceed the
tensile strength of the concrete. Vertical cracks occur first due to flexural stresses
and they start at the bottom of the beam where the flexural stresses are the largest.
Next, inclined cracks occur at the end or near the support of the beam due to
combined shear and flexure. These cracks must exist before a beam fails in shear.
Some inclined cracks extended along the main reinforcement towards the support and
weakening the anchorage of the reinforcement (MacGregor & Bartlet, 2000).
21
1.5V/(bd) y v=VQ/(Ib) fx=My/I
Figure 2.4: Flexural and shear stresses (Pillai et al., 1999)
V f1 f2 fx V V fx ≡ α V f2 f1 = ft
Figure 2.5: Flexural and shear stress and principal stresses (Pillai et al., 1999)
Figure 2.6: Stress trajectories (Pillai et al., 1999)
Figure 2.7: Potential crack pattern (Pillai et al., 1999)
90º
22
(Equation 2.3)
2.7.2 Behaviour of beam without stirrups
Figure 2.8 shows the shear mechanism acting in a beam without stirrups. A change
in moment (thus shear transfer along the shear-span), can be by one of two
mechanisms (Stratford & Burgoyne, 2003):
i) Variation in the magnitude of the internal actions
ii) Variation in the lever-arm between the actions
Beam action describes shear transfer by changes in the magnitude of the
compression-zone concrete and flexural reinforcement actions, with a constant lever-
arm, requiring load-transfer between the two forces (ACI Committee 440, 2006).
Wang et al. (2000) describe the transfer of shear in reinforced concrete without shear
reinforcement by a combination of the following mechanisms:
i) Shear resistance of the uncracked concrete, Vc
ii) Aggregate interlock force, Va tangentially along a crack
iii) Dowel action, Vd (the resistance of the longitudinal reinforcement to a
transverse force
iv) Arch action (on deep beams)
Figure 2.8: Shear mechanism acting in a beam without stirrups (Wang et al., 2007)
The equilibrium of vertical forces is:
푉 = 푉 + 푉 + 푉
Tensile Force
Vd (Dowel Force)
Va (Aggregate Interlock or Interface Shear)
Vc (Shear Resistance) Compressive Force
23
(Equation 2.4)
(Equation 2.5)
(Equation 2.6)
(Equation 2.7)
The proportion of shear transferred by the various mechanisms are in the range of
20% to 40% by the uncracked concrete, 33% to 50% by the aggregate interlock and
15% to 25% by the dowel action (Sinha, 2003). The equation to calculate shear
strength for beams without web reinforcement which is presented in ACI 318-08
(2008):
푉 = 푉
푉 = 1.9 푓 + 2500 푏 푑 ≤ 3.5 푓′ 푏 푑
In SI unit with f’c, in MPa, ACI 318-08 gives:
푉 = 0.16 푓 + 17 푏 푑 ≤ 0.29 푓′ 푏 푑 The equation is then simplified where the second term will be equaled to about 0.008 푓′ :
푉 = 0.167 푓′ 푏 푑
2.7.3 Factors affecting the shear strength of beams without stirrups MacGregor & Bartlett (2000) have indicated that there are five variables affecting the
shear strength of a beam without stirrups:
i) Tensile strength of concrete
The inclined cracking load is a function of the tensile strength of concrete. A
flexural crack which precedes the inclined cracks disrupts the elastic stress to
a level that an inclined crack occurs at a principal tensile stress.
ii) Longitudinal reinforcement ratio, ρw
Based on the equation of 휌 = 퐴 푏⁄ 푑, when the steel reinforcement ratio
is small, flexural cracks extend higher into the beam and therefore open wider
than the case for large values of ρw and as a results, inclined cracks occur
earlier.
iii) Shear span to depth ratio, av/d
Deep Beams (푎 푑⁄ ≤ 1): For deep beams, the possible modes of failure
includes an anchorage failure, crushing failure at the reactions, flexural
failure either from a crushing of concrete near the top of the arch or a yielding
24
of the tension reinforcement and a failure of the arch rib. The shear stress for
deep beams has the predominant effect.
Short Beams (1 < 푎 푑⁄ ≤ 2.5): Short beams have a shear strength that
exceeds the inclined cracking strength where as the load increases, after the
flexural-shear crack develops, the crack extends further into the compression
zone. The crack also propagates as a secondary crack towards the tension
reinforcement and then progresses horizontally along the reinforcement.
Failure of the beams is either by an anchorage failure at the tension
reinforcement or by a crushing failure in the concrete near the compression
zone.
Intermediate Length Beams (2.5 < 푎 푑⁄ ≤ 6): For this group, the vertical
flexural cracks are the first to form and followed by the inclined flexural-
shear cracks. This is the usual category for beam design. The beam may fail
either by shear or flexure. If shear reinforcement is not provided, the cracks
propagate rapidly to the top of beam, failure occurs suddenly and termed as
diagonal tension failure. If shear reinforcement is provided, load can be
carried until failure occurs in shear tension mode (yielding of stirrups) or
shear compression mode or flexural mode.
Long Beams (푎 푑⁄ > 6): For this type of beams, the failure starts with
yielding of tension reinforcement and ends by crushing of the concrete at the
section of maximum bending moment. The strength of the beam depends
entirely on the magnitude of the maximum bending moment and is not
affected by the size of the shear force. For the design of all beams except
deep beams, the shear strength is assumed to be reached when the inclined
crack forms (Wang et al., 2007). Figure 2.9 shows the effect of shear span to
effective depth ratio on shear strength of beam without stirrups (Sinha, 2003).
267
REFERENCES ACI Committee 440 (2002). Guide for the Design and Construction of Externally
Bonded FRP Systems for Strengthening Concrete Structures. Farmington Hills, USA: American Concrete Institute
ACI Committee 440 (2006). Report on Fiber-Reinforced Polymer (FRP)
Reinforcement for Concrete Structures. Farmington Hills, USA: American Concrete Institute
ACI Committee 440 (2008). Guide for the Design and Construction of Externally
Bonded FRP Systems for Strengthening Concrete Structures. Farmington Hills, USA: American Concrete Institute
Adhikary, B.B., Mutsuyoshi, H. & Ashraf, M. (2004) Shear Strengthening of
Reinforced Concrete Beams using Fiber Reinforced Polymer Sheets with Bonded Anchorage. ACI Structural Journal. 101(5), pp. 660-668
Adhikary, B.B. & Mutsuyoshi, H. (2004) Behavior of Concrete Beams Strengthened
in Shear with Carbon-Fiber Sheets. Journal of Composites for Construction. 8(3), pp. 258 - 264
Ashour, A.F., El-Refaie, S.A. & Garrity, S.W. (2004). Flexural Strengthening of RC
Continuous Beams using CFRP Laminates. Cement and Concrete Composites. 26, pp. 765 - 775
Balaguru, P., Nanni, A. & Giancaspro. J. (2009). FRP Composites for Reinforced
and Prestress Concrete Structures. USA: Taylor & Francis Group. Belarbi, A. (2011). Behaviour of Full-scale RC-T Beams Strengthened in Shear with
Externally Bonded FRP Sheets. Constr Build Mater, doi:10.1016/j.conbuildmat.2010.11.102
Bousselham, A. & Chaallal, O. (2008). Mechanisms of Shear Resistance of Concrete
Beams Strengthened in Shear with Externally Bonded FRP. Journal of Composites for Construction. 12(5), pp. 499 – 512
Bousselham A. & Chaallal O. (2004). Shear Strengthening Reinforced Concrete
Beams with Fiber-Reinforced Polymer: Assessment of Influencing Parameters and Required Research. ACI Structural Journal. 101(2), pp. 210 - 227
Cao, S.Y., Chen, J.F., Teng, J.G., Hao, Z & Chen J. (2005). Debonding in RC Beams
Shear Strengthened with Complete FRP Wraps. Journal of Composites for Construction. 9(5), pp. 417 - 428
Cervenka, V., Jendele, L. & Cervenka, J. (2001). ATENA Program Documentation
Part 1: Theory. Prague, Czech Republic: Cervenka Consulting Ltd.
268
Chaallal, O. Nollet, M.J. & Perraton, D. (1998). Shear Strengthening of RC Beams by Externally Bonded Side CFRP Strips. Journal of Composites for Construction. 2(2), pp. 111 - 113
Chajes, M.J., Januszka, T.F., Mertz, D.R., Thomson, T.A.J. & Finch, W.W.J (1995).
Shear Strengthening of Reinforced Concrete Beams using Externally Applied Composite Fabrics. ACI Structural Journal. 92(2), pp. 295 – 303
Chen, J.F. & Teng, J.G. (2003). Shear Capacity of FRP-Strengthened RC Beams :
FRP Debonding. Construction and Building Materials 17, pp. 27 - 42 Colalillo, M.A. & Sheikh, S.A. (2011). Seismic Retrofit of Shear-critical Reinforced
Concrete Beams using CFRP. Constr Build Mater, doi:10.1016/j.conbuildmat. 2010.12.065
Cusson,R & Xi, Y. (2002). The Behaviour of Fiber-Reinforced Polymer
Reinforcement in Low Temperature Environmental Climates. Colorado: University of Colorado.
El-Ariss, B (2007). Behaviour of Beams with Dowel Action. Engineering Structures.
29, pp. 899 - 903 El-Refaie, S.A., Ashour, A.F. & Garrity, S.W. (2001). Strengtheing of Reinforced
Concrete Continuous Beams with CFRP Composites. Proceedings of the International Conference on Structural Engineering, Mechanics and Computation. Cape Town, South Africa: Elsevier. pp. 1591 - 1598
El-Sayed, A.K. & Soudki, K. (2010). Evaluation of Shear Design Equation of
Concrete Beam with FRP Reinforcement. Journal of Composites for Construction 15(1), pp. 9-20
fib. (2001). Externally Bonded FRP Reinforcement for RC Structures. Switzerland:
International Federation for Structural Concrete. Gamage, K., Al-Mahaidi, R., & Wong, B. (2010). FE Modelling of CFRP-Concrete
Interface Subjected to Cyclic Temperature, Humidity and Mechanical Stress. Composite Structures, 92(4), pp. 826-834.
Godat, A., Neale, K.W. & Labossiere, P. (2007). Numerical Modeling of FRP Shear-
Strengthened Reinforced Concrete Beams. Journal of Composites for Construction. 11(6), pp. 640 - 649
Grace, N. F., Soliman, A.K. Abdel Sayed, G & Saleh K.R. (1998). Behaviour and
Ductility of Simply and Continuous FRP Reinforced Beams. Journal of Composites for Construction. 2(4), pp. 186 - 194
Gravina, R.J. & Smith, S.T. (2008). Flexural Behaviour of Indeterminate Concrete
Beams Reinforced with FRP Bars. Engineering Structures 30(9), pp. 2370-2380
269
Hanus, J.P, Bank, L.C. & Oliva, M.G. (2009). Combined Loading of a Bridge Deck Reinforced with a Structural FRP Stay-in-Place From. Construction and Building Materials 23(4), pp. 1605-1619.
Ianniruberto, U. & Imbimbo, M. (2004). Role of Fiber Reinforced Plastic Sheets in
Shear Response of Reinforced Concrete Beams: Experimental and Analytical Results. Journal of Composites for Construction. 8(5), pp. 415 - 424
Jayaprakash J, Abdul Aziz AA, Ashrabov AA & Abang Abdullah AA. (2008). Shear
Capacity of Pre-cracked and Non Pre-cracked Reinforced Concrete Shear Beams with Externally Bonded Bi-directional CFRP Strips. Construction and Building Materials 22, pp. 1148 - 1165
Khalifa, A. & Nanni, A. (2002). Rehabilitation of Rectangular Simply Supported RC
Beams with Shear Deficiencies using CFRP Composites. Construction and Building Materials 16, pp. 135-146
Khalifa, A. & Nanni, A. (2000). Improving Shear Capacity of Existing RC T-Section
Beams using CFRP Composites. Cement and Concrete Composites. 22, pp. 165-174
Khalifa, A., Belarbi, A & Nanni, A. (2000). Shear Performance of RC Members
Strengthened with Externally Bonded FRP Wraps. Proceeding of 12th World Conference on Earthquake Engineering. Auckland, New Zealand: American Concrete Institute. pp. 10 - 18
Khalifa, A., Tumialan, G., Nanni, A. & Belarbi, A. (1999). Shear Strengthening of
Continuous RC Beams using Externally Bonded CFRP Sheets. Proceedings of 4th International Symposium on FRP for Reinforcement of Concrete Structures (FRPRCS4). Baltimore: American Concrete Institute. pp. 995 - 1008
Khalifa, A. Gold, W.J., Nanni, A. & Abdel Aziz, M.I. (1998). Contribution of
Externally Bonded FRP to Shear Capacity of RC Flexural Members. Journal of Composites for Construction. 2(4), pp. 195 - 202
Kim, G., Sim, J. & Oh, H. (2008). Shear Strength of Strengthened RC Beams with
FRPs in Shear. Construction and Building Materials. 22, pp. 1261-1270. Kim, S.W. & Vecchio, F.J. (2008). Modeling of Shear-Critical Reinforced Concrete
Structures Repaired with Fiber-Reinforced Polymer Composites. Journal of Structural Engineering. 134(8), pp. 1288 - 1299
Kishi, N., Zhang, G., & Mikami, H. (2005). Numerical Cracking and Debonding
Analysis of RC Beams Reinforced with FRP Sheet. Journal of Composites for Construction, 9(6), pp. 507-514.
Kodur, V.K.R. & Baingo, D. (1999). Evaluation of Fire Resistancee of FRP-
reinforced Concrete Slabs. pp. 927-937
270
Larbi, A. S., Agbossou, A., & Hamelin, P. (2012). Experimental and Numerical Investigations about Textile-Reinforced Concrete and Hybrid Solutions for Repairing and/or Strengthening Reinforced Concrete Beams. Composite Structures. 99, pp. 152-162
Lee, J-Y, Hwang, H-B & Doh, J-H (2012). Effective Strain of RC Beams
Strengthened in Shear with FRP. Composites: Part B. 43, pp. 754-765. Lee, H.K., Kim, B.R. & Ha, S.K. (2008). Numerical Evaluation of Shear
Strengthening Performance of CFRP Sheets/Strips and Sprayed Epoxy Coating Repair Systems. Composites: Part B. 39, pp. 851 - 862
Leung, C.K.Y. & Pan, J (2005). Effect on Concrete Composition on FRP/Concrete
Bond Capacity. Proceedings of the International Symposium on Bond Behaviour of FRP in Structure. HKUST
Li. A, Diagana, C. & Delmas, Y. (2002). Shear Strengthening Effect by Bonded
Composite Fabrics on RC Beams. Composites: Part B. 33, pp. 225-239 Li, G., Maricherla, D., Singh, K., Pang, S.S. & John, M. (2006). Effect of Fiber
Orientation on the Structural Behavior of FRP Wrapped Concrete Cylinders. Composite Structures 74, pp. 475-483
Li, L.J., Guo, Y.C., Liu, F. & Bungey, J.H. (2006). An Experimental and Numerical
Study of the Effect of Thickness and Length of CFRP on Performance of Repaired Reinforced Concrete Beams. Construction and Building Materials 20, pp. 901 - 909
MacGregor, J.G. & Bartlet, F.M. (2000). Reinforced Concrete-Mechanics and
Design. Canada, Ontario: Prentice-Hall Mohamad, N. (2010). The Structural Behaviour of Precast Lightweight Foamed
Concrete Sandwich Panels as a Load-bearing Wall. Universiti Teknologi Malaysia: Ph.D. Thesis.
Monti, G. & Liotta, M.A. (2007). Tests and Design Equations for FRP-Strengthening
in Shear. Construction and Building Materials 21, pp. 799-809 Mosallam, A. S., & Banerjee, S. (2007). Shear Enhancement of Reinforced Concrete
Beams Strengthened with FRP Composite Laminates. Composites Part B: Engineering, 38(5), pp. 781-793.
Norris, T., Saadatmanesh, H. & Ehsani, M.R. (1997). Shear and Flexural
Strengthening of R/C Beams with Carbon Fiber Sheets. Journal of Structural Engineering. 123(7), pp. 903 – 911
Pellegrino, C & Modena, C. (2006). Fibre-Reinforced Polymer Shear Strengthening
of Reinforced Concrete Beams: Experimental Study and Analytical Modeling. ACI Structural Journal. 103(5), pp 720-728
271
Pham, H. B., Al-Mahaidi, R., & Saouma, V. (2006). Modelling of CFRP–Concrete Bond using Smeared and Discrete Cracks. Composite structures,75(1), pp. 145-150.
Pillai, S.U., Kirk, D.W. & Erki, M.A. (1999). Reinforced Concrete Design. Canada:
McGraw-Hill Ryerson Ltd. Razaqpur, A Ghani, Isgor & O Burkan (2006). Proposed Shear Design Method for
FRP-Reinforced Concrete Members without Stirrups. ACI Materials Journal Sika Kimia Sdn. Bhd. (2007). Sika Wrap®- 160 BI-C/15. Woven Carbon Fiber
Fabric for Structural Strengthening. Switzerland: Sika Manufacturer’s Product Data Sheet.
Sika Kimia Sdn. Bhd. (2007). Sika Wrap®-330. 2-Party Epoxy Impregnation Resin.
Switzerland: Sika Manufacturer’s Product Data Sheet. Sinha, S.N. (2002). Reinforced Concrete Design. 2nd ed. Tata McGraw-Hill. Stratford, T. & Burgoyne, C (2003). Shear Analysis of Concrete with Brittle
Reinforcement. Journal of Composites for Construction, 7(4), pp. 323-330 Taljsten, B. (2003). Strengthening Concrete Beams for Shear with CFRP Sheets.
Construction and Building Materials 17, pp. 15-26 Taljsten, B. & Blanksvard, T. (2007). Mineral-Based Bonding of Carbon FRP to
Strengthen Concrete Structures. Journal of Composites for Construction. 11(2), pp. 120-128
Triantafillou, T.C. & Antonopoulus C.P. (2000). Design of Concrete Flexural
Members Strengthened in Shear with FRP. Journal of Composites for Construction. 4(4), pp. 198 - 205
Triantafilliou T.C. (1998). Shear Strengthening of Reinforced Concrete Beams using
Epoxy-Bonded FRP Composites. ACI Structural Journal. 95(2), pp. 107 - 115
Wang, C.K., Salmon, C.G. & Pincheira, J.A. (2007). Reinforced Concrete Design. 7th
ed. New Jersey, USA: John Wiley. Wu, Z., Yuan, H., Asakura, T., Yoshizawa, H., Kobayashi, A., Kojima, Y. & Ahmed,
E. (2005). Peeling Behavior and Spalling Resistance of Bonded Bidirectional Fiber Reinforced Polymer Sheets. Journal of Composites for Construction. 9(3), pp. 214 - 226
Youakim, S.A. & Karbhari, V.M. (2006). A Simplified Method for Prediction of
Long-Term Prestress Loss in Post-Tensioned Concrete Bridges. San Diego, California, USA: University of California
272
Zhang, Zhicao & Hsu, C.T.T. (2005). Shear Strengthening of Reinforced Concrete Beams Using Carbon-Fiber-Reinforced Polymer Laminates. Journal of Composites for Construction. 9(2), pp. 158 - 169
Zou, P.X. (2003). Flexural Behaviour and Deformability of Fiber Reinforced
Polymer Prestressed Concrete Beam. Journal of Composites for Construction, 7(4), pp. 275-284